6TH INTERNATIONAL CONFERENCE ON WWER FUEL PERFORMANCE, MODELLING AND EXPERIMENTAL SUPPORT, 19 - 23 September 2005, Albena Congress Center, Bulgaria
Institute of Atomic Energy, Otwock-Świerk 05-400, Poland, E-mail: [email protected]
It is generally accepted that most of the insoluble inert gas atoms Xe and Kr produced during fissioning are retained in the fuel irradiated at a temperature lower than the threshold. Experimental data imply that we can assume that after irradiation exposure in excess of 1018 fissions/cm3 the single gas atom diffusion can be disregarded in description of fission gas behaviour. It is assumed that the vicinity of the fission fragment trajectory is the place of intensive irradiation induced chemical interaction of the fission gas products with UO2. Significant part of fission gas product is thus expected to be chemically bound in the matrix of UO2. From the moment of discovering the rare gases (helium, neon, argon, krypton, xenon and radon) at the end of XIX century until to the beginning of sixties years of XX century it was considered that the noble gases are chemically inactive. The nobility of rare gases started to deteriorate after when the first xenon compound was found by Barlett in 1962. Barlet showed that the noble gases are capable of forming what one could consider as normal chemical compounds, compelling chemists to readjust considerably their thinking regarding these elements. In a burst of activity in the years that followed, a number of compounds of noble gases have been reported. Experiments with mixture of noble gases, coupled with theoretical calculations, provide strong evidence for direct bonds between Ar, Kr, or Xe atoms and the U atom of the CUO molecule. 2+ Because of its positive charge, the UO2 ion, which is isoelectronic with CUO, should form even stronger bonds with noble gas atoms, which could lead to a growing number of complexes that contain direct noble gas – to –actinide bonds. Considering the huge amount of gas immobilised in the UO2 fuel the solution process and in consequence the re-solution process of rare gases is to be replaced by the chemical bonding process. This explains the fission gas accumulation in the irradiated UO2 fuel.
1 1. Introduction
It is generally accepted that most of the insoluble inert gas atoms Xe and Kr produced during fissioning are retained in the fuel irradiated at a temperature lower than the threshold [1-11]. Some authors [1-7] assume random diffusion of gas atoms to grain boundaries and consider the effect of trapping the atoms at inter-granular bubbles until saturation occurs. Others [12-13] confirmed that bubbles tend to concentrate in the grain boundaries during irradiation. Likewise, some authors [8-11] further assume that most of the gas atoms are retained in solution in the matrix of grains being there immobilised or are precipitated into small fission gas bubbles. In a very early publication (1964) in Journal of Nuclear Materials MacEwan and Stevens  in the work “Xenon Diffusion in UO2 (some complicating factors)” have proved experimentally that an appreciable fraction (F) of the fission xenon was immobilised after irradiation exposure in excess of 1015 fissions/cm3. In fig. 1 are plotted the fractions, F, of trapped xenon in the specimens for both the sintered and single-crystal specimens. A tolerable fit to each set of results was obtained with an exponential law expression, A[1-exp(-αn], where n was the number of fission events/cm3 and A and α are constants.
Fig.1. A plot showing how the fraction of the fission xenon trapped after annealing for a short period at 1400 o C varies as a function of the prior irradiation exposure .
It is clearly seen from the fig. 1 that after irradiation exposure in excess of 1018 3 fissions/cm both for the single crystal specimen and the sintered UO2 significant portion of xenon is immobilised namely 95 % and 78 % respectively. MacEwan and Stevens underlined that if it were assumed that all xenon was free to migrate, the diffusion coefficient for xenon decreased by a factor of 1000 for the single crystal UO2 and by a factor of 20 for the sintered UO2. Several years later in 1972 Samsonov and Fray  have carried out an in-pile investigation from 1 to 400 MWD/t(U). They observed releases of 3 isotopes of xenon and obtained different decreases for the apparent diffusion coefficient: by a factor of 5 to 6 powers of ten for Xe133, 2 to 4 powers for Xe135 and 1 to 3 powers for Xe138. They also observed saturation after about irradiation exposure in excess of 1018 fissions/ cm3. This is illustrated below in fig. 2. A remarkable fact is that the values of apparent diffusion coefficients of Xe133, Xe135 and Xe138 after irradiation beside that the coefficients decreased but also its order is in reverse.
2 Fig. 2. Dependence of apparent diffusion coefficient on burn-up .
The above mentioned experimental data imply that we can assume that after irradiation exposure in excess of 1018 fissions/cm3 the single gas atom diffusion can be disregarded in description of fission gas behaviour. It means that significant fraction of fission gas products is not available for diffusion. This is a general observation for the whole temperature range of UO2 fuel that is exploited in the light water reactors (LWR). The above well documented assumption implies that a single gas atom diffusion model cannot be used to estimate the amount of fission gas that will be released from UO2 during irradiation Out of pile experiments show that during annealing the irradiated UO2 samples bursts of fission gas release occur . After a small burst release at relatively low temperature, a large burst release appears at high temperature. Fig. 3 shows the release of 85Kr for a fuel burn-up of 16 and 28 GWd/tU together with the temperature history, heating to 1000 °C at the rate of 100 °C/min and then raising by steps of 100 °C at the same rate and holding at each temperature. In the case of the 16 GWd/t specimen, after a straight release at each temperature rise to 1500, a large burst release appears from 1500 to 1600 °C. For the 28 GWd/t specimen, prior to the large burst releases at the temperatures above 1500 °C a small burst release around 200~300 °C appears, which corresponds to the fractional release of about 1.5%. This low temperature burst release is probably due to the occurrence of intergranular microcracks induced by thermal shock .
3 Fig. 3. Kr85 release on stepwise temperature ramp .
Fig. 4. Burn-up dependence of critical temperature for onset of burst release .
4 The critical temperature for the onset of the high temperature burst release is plotted against fuel burn-up in Fig. 4. The diagram indicated that the bursts release temperature becomes lower with increasing burn-up. The same tendency has been reported by Vitanza et al. , who measured the fuel centreline temperature of instrumented fuel rods in the Halden Reactor. The fractional fission gas release of the rods was above 1%. This burn-up dependence of burst release temperature is attributable to the increases of fission gas inventory in the grain boundaries and the density of the grain boundary bubbles at higher burn-ups. The Vitanza’s curve is shown in Fig. 5.
Fig. 5 Incubation time (burn-up) as a function of the centre temperature .
The critical temperature for high temperature burst release is about 1800 0C for low burn-up ( about 7 MWd/kgU ) and decreases to about 1500 0C for high burn-up ( 30 MWd/ kgU ). The point defects induced by radiation begin to recover at 450 – 650 0C and are completely almost recovered above 850 0C, while defect clusters of dislocations and small intragranular bubbles require 1150 – 1450 0C . Thermal recovery of radiation defects and microstructure change in irradiated UO2 fuels studied by X – ray diffraction and transmission electron microscopy lead to the conclusion that the gas release kinetics from irradiated UO2 is determined by the kinetics of thermal recovery of the radiation induced defects. If the point defects, defect clusters of dislocations and small intra-granular bubbles are thermally recovered at the temperatures below 1450 0C, a natural question concerns nature of forces which immobilise the noble gases. Hence an additional trapping process of inert gas atoms with the uranium dioxide material is suspected to occur. The process of strong binding of the fission gas fragments with the irradiation defects is described in the literature as a process of chemical interaction with UO2. It is important to remind here the MacInnes and Winter’s remark  that the crucial assumption concerning the fuel for long time was that the fission gases and volatile fission products, principally Xe and Cs, have no effect on the chemical state of the fuel. This seems reasonable if these fission products have been released from the fuel, but its validity must be called into question if a fraction is distributed within the grains as single atoms. Since these atoms tend to precipitate from the fuel, they will interact with the thermally-generated point defects in the UO2 lattice.
5 It is assumed further that the vicinity of the fission fragment trajectory is the place of intensive irradiation induced chemical interaction of the fission gas products with UO2 . We can further assume that above a limiting value of fission fluency (burn-up) a more intensive process of irradiation induced chemical interaction occurs. Significant part of fission gas product is thus expected to be chemically bound in the matrix of UO2.
2. Chemical activity of noble gases
From the moment of discovering the rare gases (helium, neon, argon, krypton, xenon and radon) at the end of XIX century until to the beginning of sixties years of XX century it was considered that the noble gases are chemically inactive. The nobility of rare gases started to deteriorate after the first xenon compound was found by Barlett in 1962 . Barlet showed that the noble gases are capable of forming what one could consider as normal chemical compounds, compelling chemists to readjust considerably their thinking regarding these elements.
2.1. The general noble gases characteristic.
The ability of the noble gases to combine with other atoms is relatively limited because their closed–shell electronic structures are extremely stable. This ability would be expected to increase with decreasing ionisation energy and decreasing energy promotion to states with unpaired electrons. This is clearly seen in the Table 1 [19-20] presenting the basic chemical and physical properties of the noble gases. Except the helium, which has the outer shell configuration 1s2, the other elements of the periodic group have the outer shell configuration s2p6. The helium group gases do not form stable positive ions because of high ionisation energy. The noble gases show negative electron affinity and that is why they do not form anions. In the standard conditions the noble gases occur in the atomic form since they do not attach and do not give up the electrons and because of that they do not show trend to form chemical bonds.
Table 1. Chemical and physical properties of the noble gases [19-20]
Element Outer shell First Second Promotion Electron Boiling % by configuration ionisation ionisation energy affinity point volume in energy energy np6→np5(n+1)s1 [eV] [oC] the [eV] [eV] [eV] atmosphere 2He 1s2 24.59 54.42 19.8 0.077 -268.9 5.2⋅10-4 10 2 6 Ne 2s 2p 21.56 40.96 16.6 -0.40 -246.0 1.8⋅10-3 18Ar 3s23p6 15.76 27.63 11.5 -0.36 -185.9 0.93 36 2 6 Kr 4s 4p 14.00 24.36 9.9 -0.40 -153.2 1.1⋅10-3 54 2 6 Xe 5s 5p 12.13 20.98 8.3 -0.42 -108.1 8.7 10-6 86 2 6 ⋅ Rn 6s 6p 10.75 18.00 6.8 − -62.0 vestigial
It is known that the noble gases can be trapped in clathrates. In the clathrates, atoms of noble gases are trapped in the lattice of the host substance. There are no chemical bonds between the gas atoms and the surrounding atoms in the usual sense, but instead, only weak Van der Waal forces. The element therefore escapes when the host crystal melts or dissolves [19-21]. The rare gases form one of the most abundant classes of constituents of our Universe. The beautiful octet rule led scientists to accept the nonreactivity of rare gases until 1933, when Linus Pauling suggested  from considerations of ionic radii of different elements
6 that molecules like XeF6 and KrF6 and perhaps unstable compounds XeF8 and H4XeO6 should be preparable. However, attempts to synthesise rare-gas –containing molecules were not successful at that time . It took about 30 years until the first rare-gas-containing chemical compound was found. + - After the observation that O2 reacts with PtF6 to give the compound [O2 ][PtF6 ], Neil Barlet  recognised that since the first ionisation energy of Xe (Xe→Xe+ 12.3 eV≡1169kJ/mol) is + almost identical with that of molecule O2 (O2→O2 1177 kJ/mole), an analogous reaction should occur with Xe. He obtained a red solid by reaction of Xe with PtF6 in the room temperature: + - Xe + PtF6 → Xe [PtF6]
Present knowledge indicates that the reaction is more complicated and that the xenon oxidation sequence is following :
25oC 60oC + - + - Xe + 2PtF6 ⎯⎯→[XeF] [PtF6] + PtF3 ⎯⎯→ [XeF] [Pt2F11]
The key idea for this discovery was the similar ionisation potentials of O2 and Xe.
2.2. Examples of rare gas compounds
In a burst of activity in the years that followed after the discovery of the first halogen compound, a number of compounds of noble gases have been reported, especially with xenon. It is observed, that the rare gases make reaction with the most electronegative elements, such as fluorine and oxygen. Later it has been shown that Xe (sometimes Kr) form bonds also with other non-metals, and even with some metals. While many of these can be regarded as metastable species, several are actually thermodynamically stable compounds and can be obtained commercially. Very shortly after the discovery of rare compounds, specialists made considerable contributions to the understanding of their chemistry . Xenon reacts directly only with F2, but compounds in oxidation states from II to VIII are known, some of which are exceedingly stable and can be obtained in large quantities. The more important compounds and some of their properties are given in Table 2.
Table 2.Principle xenon compounds 
Oxidation Compound Form Mp Structure Remarks state [oC] II XeF2 Colorless crystals 129 Linear Very solubble IV XeF4 Colorless crystals 117 Square Stable VI XeF6 Colorless crystals 49.6 Complex Stable CsXeF7 Colorless solid o Cs2XeF8 Yellow solid Stable to 400 C XeOF4 Colorless liquid -46 Octahedral Stable XeO2F2 Colorless crystals 31 Metastable XeO3 Colorless crystals Explosive, stable in solution
VII XeO4 Colorless gas -35.9 Tetrahedral Highly explosive XeO3F2 Colorless gas -54.1
7 When xenon and fluorine are mixed together, only a small amount of energy by heating up the mixture is needed to initiate the formation of fluorides. According to the amount of reagents there can be formed three different products: XeF2, XeF4 and XeF6 [19,20,25]. Formation of bonds in these three fluorides can be explained by the theory of covalent bonds . It is worth to underline that xenon difluoride obtained commercially has found a relatively widespread use as a fluorinating agent and has useful applications in semiconductor processing for etching silicon. The three fluorides XeF2, XeF4 and XeF6 can be used to form anionic species in reactions such as .
+ - XeF4 + NaF → Na [XeF5] + - XeF6 + CsF → Cs [XeF7] + - 2XeF6 + NO2F → NO2 [Xe2F13] + - 2XeF2 + AsF5 → [Xe2F3] [AsF6] + - XeF2 + RuF5 → [XeF] [RuF6] + XeF2 + 2SbF5 → [XeF] [Sb2F11]
A group of rare-gas molecules, krypton and xenon hydrides HRgY, where Rg is a rare gas and Y is an electronegative fragment, have been identified in low-temperatures matrices . The first observed HRgY compounds were triatomic HXeY (Y = H, Cl, Br, I) and HKrCl molecules [27, 28].
`Fig. 6. The role of relativity. In the atomic AuXe+, roughly half of the Au-Xe bond strength arises from relativistic effects. V, bonding energy; R, interatomic distance (Copied from ).
Another complex compounds were obtained as HXeNCO , HXeNC , HKrCN , HXeSH , HXeOH  and HXeNCO . Pyykko recalls, that Seidel and Seppelt  take noble gas bonds a step further, reporting a bulk compound held together by covalent bonds between gold and xenon. If gold were a truly noble metal and xenon a truly noble gas, such an Au-Xe bond would be impossible. In actual fact, noble metals such as platinum and gold have a rich chemistry. It
8 has been theoretically predicted  that XeAuXe+, which has the same number of valence electrons in similar molecular orbitals as the ClAuCl- anion, should posses short, strong covalent bonds between xenon and gold. The lighter rare gases were predicted to form similar, but more weakly bound systems. The simpler diatomic species, such as AuXe+, were 2+ also predicted. The authors  characterised [AuXe4] ion, in which the Xe atoms act as electron donors to the electron-deficient Au2+ ion. Two of the predicted species, AuXe+, and XeAuXe+, have been observed experimentally by mass spectroscopy . Relativity plays a large role in stabilising these Au-Xe compounds; about half of the Au- Xe bonding energy comes from relativistic effects (see Fig. 6). The high nuclear charge of gold accelerates the 6s valence electrons to high speeds when they dive near the nucleus. In a simple picture, the consequent relativistic mass increase compresses and stabilises the valence 6s shell. This relativistic stabilisation of the 6s shell makes covalent bonds to gold anomalously strong and short . There is very interesting report on bonding between noble gas atoms and an actinide metal atom uranium. The developments began with the observation that the CUO molecule, which has been trapped in noble gas matrices, exhibits notably different spectroscopic behaviour in the presence of Ar, Kr, or Xe than in matrices of pure Ne .
Fig. 7. Potential energy curves for the 1A’ and 3A” states of CUO⋅Ar as a function of the U-Ar distance. The inset figure lower right shows the optimised structure of the 3A” state of CUO⋅Ar . The U-Ar bond length in this complex is 316 pm.(copied from )
Experiments with mixture of noble gases using the infrared spectroscopy (IR), coupled with theoretical calculations, provide strong evidence for direct bonds between Ar, Kr, or Xe atoms and the U atom of the CUO molecule . Calculations on CUO⋅Ar were carried out with the CUO molecule in its 1Σ+ (1A’) ground state and its low-lying 3Φ (3A”) excited state, where the Greek state designations are for the linear geometry of CUO, whereas the designations in parentheses are appropriate for the CUO⋅Ar molecule. It is found that CUO⋅Ar is a planar molecule with a 3A” ground state in which a bent CUO fragment is bound to the Ar atom primarily through the U atom (see Fig.
9 7). The Ar atom interacts most significantly with the U and C atoms. Figure 7 shows a slice through the calculated potential energy surfaces of the 3A” ground state and 1A’ excited state of CUO⋅Ar as a function of the U-Ar distance. Orbital analysis of the calculations on 3A” and 1A’ CUO⋅Ar indicates that, the Ar atom serves as a base that donates electron density into an empty U 6d orbital . The density functional theory (DFT) calculations predict that the interaction of a Kr or Xe atom with CUO is stronger than that of an Ar atom. The stabilisation of the 3A” ground state of CUO⋅Kr and CUO⋅Xe are 1.1 and 3.6 kcal/mol greater than that in CUO⋅Ar, respectively. The calculated U-Kr and U-Xe distances, 324 and 330 pm, respectively, are shorter than the sums of the crystal radii (341 and 358 pm, repectively) . To explore the notion of multiple CUO⋅Arx species further, it was calculated the structures of CUO⋅Arx (x=2 to 6) complexes The theoretical results provide strong support for the binding of multiple Ar atoms to a single CUO molecule. The binding of two or more Ar atoms continues to favour the triplet form of CUO . The authors believe that the experimental and the theoretical data presented in their report  make a strong case for the interactions between the U atom of CUO and the noble gas (Ng) atoms. The U-Ng bond distances are short, and the U-Ng interaction is strong enough to 2+ change the spin state of the CUO molecules. Because of the positive charge, the UO2 ion, which is isoelectronic with CUO, should form even stronger bonds with noble gas atoms, which could lead to growing number of complexes, that contain direct noble gas – to – actinide bonds.
The examples of rare gas compounds presented above show that noble gas chemistry is much richer than it would be expected. New chemical bonds between strange bedfellows, like noble metals, actinides and noble gases, can still be found. Since the examples of rare gas compounds presented above are formed by applying the classical chemical methods, the more the noble gas spices in the conditions of neutron and fission fragments irradiation of the UO2 fuel type can be expected. This assumption is suggested by the fact that the ClXeCl has been found to form after irradiation with 501.7 nm laser light of Cl2-doped xenon matrices. It appears that after excitation of the Cl2 there is little or no barrier for the rearrangement to ClXeCl . The fission fragments are striped of about 20 electrons along most of their paths in the medium in which the fission takes place. The high positive charge of the fragments was estimated by Bohr (1940, 1941) [39-40]. He assumed that the equilibrium is reached, e.g. that the probabilities for electron capture or loss by the ion are equal when the ionic velocity and the velocity of the electrons within the ion is the same. Lamb (1940)  considered the electrons within the decelerating medium as practically free and assumed that the kinetic energy of these electrons relative to the ion is, at equilibrium, equal to the ionisation energy of the outermost electrons within the ion. Knipp and Teller (1941)  and Ozeroff (1949)  computed the fission particle charge states. The equilibrium charge states in various solids of several ions were measured in the energy range 10 – 100Mev by Leischner (1966) . Measurements on 79Br and 127I by Moak et al., (1968)  are of particular interest here, since these two ions may be considered as typical fission fragments. Their most probable charge states are plotted versus ion energy in Figs 8 and 9. We see that charges of the two groups of fission fragments are about 22 at the beginning of their paths and decrease slowly, and are still 10 at 10 Mev, e.g. near the end of their paths. Fission fragments are at the same time very energetic and highly charged particles; they interact strongly with electrons of the material losing their energy mainly by ionisation but also by elastic collisions with atoms as a whole .
10 The kinetic energy of the two fragments is about 160 MeV. . But the energy ν that each fission event delivers directly to the lattice of the irradiated material via atomic collisions does not exceed 10 MeV . The energy given directly to the lattice, via atomic collisions, is 5,4 ± 1.5 MeV for the median heavy fragment, and only 3.3 ± 1.5 MeV for the median light fragment. It is therefore assumed that each fission event dissipates roughly 10 MeV (from 5 to 15 MeV) through atomic collisions in fissile materials .
Fig. 8. Most probable charge state for 79Br ions in solids versus ion energy [44.
Fig. 9. Most probable charge state for 127I ions in solids versus ion energy .
95 % of the initial fission fragment energy is finally lost through ionisation processes, e.g. to electrons with the huge rate of 5 to 10 MeV energy loss per atomic distance. Whatever the
11 material, this energy is ultimately converted into heat, but there is an important difference in behaviour between a metal and an insulator. In an insulator (e.g. UO2), energy lost by ionisation can only diffuse through the slow and weak electron-phonon and phonon-phonon interactions. Weak because electrons diffused by phonons loose only a small amount of energy in each collision. Slow because the relaxation times of electron-phonon and especially phonon-phonon collisions are slow. Therefore ionisation may induce very large thermal effects in insulators (thermal spike) . It is interesting to know the maximum number of Frenkel pairs created by one fission event. The number of Frenkel pairs created is directly connected to the energy given to the lattice by each fission event Its approximate value is N = ν/(2Ed), where Ed is the displacement threshold energy, ν is indeed the energy actually given to the lattice. This means that ν is not the sum of all primary energies but the sum of all primary energies minus the fraction of these energies lost by ionisation. But of course, some of these defects created are immediately annealed, even if the irradiated lattice is completely frozen. This anneal, very difficult to estimate, is due to recombination of opposite defects, either athermally by overlapping of damaged regions or by spontaneous recombination of very close Frenkel pairs, or thermally in thermal spikes. A commonly accepted value of Ed is 25 eV. So the maximum number of Frenkel pairs created by one fission event is then 200 000  In UO2 dislocations are observed very soon after the beginning of the irradiation. o 16 -3 Dislocation loops about 25 A in diameter and with density of 10 cm are seen ofor a dose of 4.3 x 1015 fissions/cm3. After 6x1016 fissions/cm3, the average diameter is 100 A . When the 16 3 dose increases, the loop density in UO2 becomes saturated at about 2x10 fissions/cm but the average loop size increases. Whapham and Sheldon in 1965 described the nature of point defect clusters in UO2 . They concluded that vacancy clusters are observed only after 1020 fissions/cm3 while the clusters observed after 4.3x1015 or 3.7x1017 fissions/cm3 are interstitial dislocation loops. As a conclusion, displacement cascades in fissile materials are characterised by the generation of a very high point defects concentration, immediately followed by an intense thermal spike. Keeping in mind that the UO2 fuel is highly defected, ionised with very energetic and highly charged fission fragments, it appears that during irradiation there is little or no barrier for the formation of rare gas atoms compounds with the UO2 molecule and fission products. There would be a strong interaction between the U atom of UO2, fission products and the noble gas (Ng) atoms. This further implies that significant part of the fission fragments after dissipating all their energy and stopping in the material being still highly ionised at the end of their paths react chemically with the fuel. Fission products are frequently divided into four general categories: noble gases, volatile elements, semi-volatiles, and non-volatiles. About 300 different fission products exist in a nuclear reactor core. The rare gases Xenon (Xe) and to a lesser extent Krypton (Kr), are two of the more abundant fission products. About 15% of fission products are rare gases; Xe (90%) and Kr (10%). It is worth to be noted that the inert gases Kr and Xe are practically not formed directly by fission, but originate by β-decays from the precursors. Se85, Se87, Br88, and Br89 are precursors for the krypton and Sn131, Sn132, Sb133, Sb134, Te135, I137, I138 and I139 are the precursors for the xenon. That is why the prompt fission yield for the Kr85m, Kr87, Kr88, Kr89 and for the Xe131, Xe133, Xe135, Xe137, Xe138 Xe139 are equal zero [48-52]. This that the inert gases Kr and Xe mostly are not formed directly by fission, but originate from the precursors imply, that the precursors which are not gas atoms can easier chemically react with the UO2 fuel than the rare gas atoms. We can assume that the precursor already chemically bond with the fuel decaying to the rare gas atom do not change the electron shell of the compound and remain chemically bonded. It means that the rare gas atoms are chemically bound with the UO2 fuel after decaying of the precursors which chemically reacted with the fuel.
12 It has been known for over a century that in the presence of an electric discharge or electron beam gas atoms become embedded into the electrodes and the walls of the vessel containing the gas . It was this observation which suggested to workers at the AECL Laboratories at Chalk River that a similar phenomena may operate on the fission gases within fuel pins during irradiation. This they proved by irradiating UO2 pellets in the presence of natural xenon. After irradiation they mass analysed the gas and took drilled cores from selected positions in the pellets and they found that indeed some of the natural xenon had been sorbed into the surface of the fuel . Whilst the gases embedded by electrical discharge were only lightly attached to solid surfaces and could easily be released by slight heating, the xenon was found to be very firmly attached to the UO2 surfaces such that only 1% of the attached gas could be removed after annealing samples for 12 hours at 1400 oC. This was the first of many experiments, which showed that the mechanism and kinetics of the phenomenon were complicated. Uranium dioxide irradiated to a burn-up greater than about 3.2 1019 fissions/cm3 between 800 and 1600 oC is always found to contain a high concentration of matrix fission-gas bubbles . The bubble nucleation density is virtually independent of both temperature and dose rate at about 1017 bubbles/cm3 [56-57]. Whapham and Sheldon  suggest, on the grounds of repeated low temperature irradiation of UO2 fuel with intermediate annealing, that the gas trapped in the bubbles may be knocked back into the matrix as a result of the action of fission fragments. This effect we assume to enhance the chemical bonding process as the gas atoms from the bubbles become ionised by the fission fragments. The phenomenon observed in the above quoted work [56-57] allows to conclude that the rate of the chemical bonding process is markedly higher than the fission gas trapping rate in the bubbles.
Keeping in mind that the gas release kinetics from irradiated UO2 is determined by the kinetics of thermal recovery of the radiation induced defects and associating it with the idea of the noble gas atoms trapped in clathrates (where no chemical bonds between gas atoms and the surrounding occur), we can postulate that in point defects, dislocation loops and gas bubbles the rare gas atoms with the closed-shell electronic structure can be immobilised. In this sense, there exists no true diffusion for the fission gas in the UO2 fuel. It appears necessary in this discussion to recall the conclusion of the panel discussion of the International Seminar on Fission Gas Behaviour in Water Reactor Fuels, held in Cadarache, France 26-29 September 2000. Namely “The notion of diffusion coefficient of the fission gas atoms should be verified and if we resign from the term re-solution then what we should assume instead”. It is very important to recall also that solubility of rare gas atoms in uranium alloys or ceramics is so low that it has not been measured. In perfect crystals, the order of magnitude of the solubility is 10-10 in the most favourable cases. This figure may be increased up to ≈ 10-5 in the vicinity of dislocations. So, considering the huge amount of gas immobilised in the UO2 fuel, the solution process and in consequence the re-solution process of rare gases is to be replaced by the irradiation enhanced chemical bonding process. This explains the huge fission gas accumulation in the irradiated UO2 fuel.
Noble gas chemistry is much richer than it would be expected.
13 Since the rare gas compounds are formed by applying the classical chemical methods, the more the noble gas spices in the conditions of neutron and fission fragments irradiation of the UO2 fuel type can be expected.
As the irradiated UO2 fuel is highly defected, ionised with very energetic and highly charged fission fragments, it appears that during irradiation there is little or no barrier for the formation of rare gas atoms compounds with the UO2 molecule and fission products. This further implies that significant part of the fission fragments after dissipating all their energy and stopping in the material being still highly ionised at the end of their paths react chemically with the fuel.
This that the inert gases Kr and Xe mostly are not formed directly by fission, but originate from the precursors imply, that the precursors which are not gas atoms can easier chemically react with the UO2 fuel than the rare gas atoms. It is assumed that the precursor already chemically bond with the fuel decaying to the rare gas atom do not change the electron shell of the compound and remain chemically bonded.
The rate of the chemical bonding process is markedly higher than the fission gas trapping rate in the bubbles.
The rare gas atoms with the closed-shell electronic structure can be immobilised in point defects, dislocation loops and gas bubbles and be released by recovery of the radiation induced defects. In this sense, there exists no true diffusion for the fission gas in the UO2 fuel.
Considering the huge amount of gas immobilised in the UO2 fuel and a very low solubility of rare gas atoms in the uranium dioxide fuel, the term re-solution is to be replaced by the irradiation-enhanced chemical bonding process. This explains the huge fission gas accumulation in the irradiated UO2 fuel.
 R. Hargreaves, D. M. Collins, J. Br. Nucl. Energy Soc. 15 (1976) 311.  R. G. Bellamy, J. B. Rich, J. Nucl. Mater. 33 (1969) 64.  H. Zimmermann; J. Nucl. Mater. 75 (1978) 154.  R. J.White, M. O. Tucker, J. Nucl. Mater. 118 (1983) 1.  T. Nakajima, H. Saito, Nucl.Engrg. Des. 101 (1987) 267.  Kenichi Ito, Ryo Iwasaki and Yoshihiko, J. Nucl. Sci. Technol. 22 (1985) 129.  J. Rest, A. W. Cronenberg , J. Nucl. Mater. 150 (1987) 203.  J. R. Mac Iwan, W. H. Stevens, J. Nucl. Mater. 11(1964) 77.  I. L. F. Ray, H. Thiele, Hj. Matzke; J. Nucl. Mater. 188 (1992) 90. T. Aoki, S. Koizumi, H. Umeharq, K. Dgotu; Fission gas release behaviour of high burn-up fuel during power ramp tests; Proceedings of a technical committee Meeting hold in Pembroke, Ontario, Canada, 28 April-1 May, 1992. M. Szuta; J. Nucl. Mater. 210(1994)178. Katsumi Une and Shinji Kashibe, J. Nucl. Sci. Technol. 27  (1990) 1002. J. Burbach, H. Zimmermann, KfK 3997, (1985).  B.W. Samsonov, A. K. Frey; SAARI – P135, Melekess, 1972.  C. Vitanza, E. Kolstad, U. Gracioni, Proc. of the American Nuclear society, Topical Meeting on Light Water Reactors Performance, Portland, Oregon, May 1979, p. 361.  Y. Nogita, K. Une, J. Nucl. Sci. Tech. 30, 900(1993).  D. A. McInnes, P. W. Winter, J. Phys. Chem. Solids Vol.49, 143(1988).  N. Barlett, Proc.Chem. Soc.. 6 (1962) 218.
14  F.A. Cotton, G. Wilkinson, C.A. Murillo, M. Bochmann; Advanced Inorganic Chemistry, John Wiley & Sons, New York 1999.  K. Łyczko, Chemistry of the noble gases; Wiadomości Chemiczne, 2002, 56,p 771-792.  L. Stein, Radichemica Acta 32,(1983)p. 163-171.  L. Pauling, J. Am. Chem. Soc. 1933,55, p.1895.  M. Pettersson, J. Lundell, M. Rasanen, Eur.J. Inorg. Chemistry 1999, p. 729-737.  M. Lorenz, M. Rasanen and V.E. Bondybey; J. Phys. Chem. A Vol. 104, No. 16 (2000), 3770 – 3774.  C.R. Bieler, K.E. Spence, K.C. Janda, J. Phys.Chem. 95, 1991, p. 5058-5064.  M. Petersson, J. Lundell, M. Rasanen; Eur. J. Inorg. Chem. 1, 1999, p. 729.  M. Petersson, J. Lundell, M. Rasanen;J. Chem. Phys., 102, 1995, p.6423.  M. Petersson, J. Lundell, M. Rasanen; J. Chem Phys. 103, 1995, p. 205.  M. Petterson, J. Lundell, L. Khriachtchev, M. Rasanen, J. Chem. Phys. 109, 1998 p. 618.  M. Petterson, J. Lundell, L. Khriachtchev, E. Isoniemi, M. Rasanen, J. Am. Chem. Soc. 120, 1998, p.7979.  M. Petterson, L. Khriachtchev, J. Lundell, , M. Rasanen, J.Am. Chem. Soc. 121, 1999, p.11904,  M. Petterson, L. Khriachtchev, J. Lundell, , S. Jolkkonen, M. Rasanen, J. Phys. Chem. A 104, 2000, p3579.  P. Pyykko; Science, Vol 290, 2000, p. 64.  S. Seidel, K. Seppelt; Science vol. 290, 2000, p. 117.  P.Pyykko, J. Am. Chem. Soc. 117, 1995, p.2067.  D. Schroder, H. Schwarz, J. Husak, P. Pyykko, Inorg. Chem. 37, 1998, p. 2067.  J. Li, B. E. Liang, L. Andrews; Science Vol. 295 (March 2002) p.2242-2245.  C.R. Bieler, K.E. Spence, K.C. Janda; J. Phys. Chem. 95, 1992, p. 5058-5064. N. Bohr, , 1940, Phys. Rev. 58, 654, N. Bohr, 1941, Phys. Rev. 59, 654, J. Knipp, E. Teller, 1941, Phys. Rev. 59, 659. J. Ozeroff, 1949, KAPL Rept,. 205, E. Leischner, 1966, UNILAC Rept. (heidelberg) 1, 66. C. D. Moak, H. O. Lutz, L. B. Bridwell, L. C. Nothcliffe, S. Datz, 1968, Phys. Rev. 176, 427.  J. Leteurtre, Y. Quere; Irradiation effects in fissile materials; North-Holland Publishing Company-Amsterdam – 1972  J. Lindhard, P. V. Thomsen, 1962, Sharing of energy dissipation between electronic and atomic motion, in : Radiation damage in solids, Vol. 1, (IAEA, Vienna) 65.  A. D. Whapham, B. E. Sheldon, 1965, Phil. Mag. 11, 1175. A. A. Grieshilov, W. W. Kolobashkin, S. I Dementev, Produkty mgnoviennovo delenia U235, U238, Pu239 v intervale 0 –1 cz, Atomizdat, Moskva,1969, a) B. S. Dzelepov, L. K. Peker, V. O. Sergeev, Schemy raspada radiaktyvnych jader, A<100, Izdatelstvo “Nauka”, Moskva, 1966. b) B. S. Dzelepov, L. K. Peker, V. O. Sergeev, Schemy raspada radiaktyvnych jader, A>100, Izdatelstvo Akademii Nauk SSSR, Moskva, 1963. M. Masalska, J. Masalski, Tablica izotopow, Postepy Techniki Jądrowej, Vademecum, Nr 16 (278), 1960, C. M.Lederer, J. M. Hollander, I. Perlman, Table of Isotopes, Sixth Edition, 1968. N. Gusev, V. Maskovitz, G. Obvincev, Gamma-izlucene radioaktyvnych iztopov i produktov delena; Gosudarstvennoe Izdatelstvo Fiziko-Matematiceskoj Literatury, Moskva, 1958.  J.A. Turnbull, Radiation Effects, Vol. 53, 1980, pp. 243-250.  W.B. Lewis, J.R. MacEwan, W.H. Stewens, R.G. Hart, Proceedings of the 3rd UN Conference on the Peaceful Uses of Atomic Energy, May (1964).
15  R.M. Cornell, J. Nucl. Mater. 38(1971)319-328  R. S. Nelson, J. Nucl. Mater. 31(1969)153. J. A. Turnbull, R. M. Cornell, J. Nucl. Mater. 41(1971)156. A. D. Whapham and B.E. Sheldon, Nucl. Appl. 2 (1966)123.